Laser-induced etching of few-layer graphene synthesized by Rapid-Chemical Vapour Deposition on Cu thin films
© Piazzi et al; licensee Springer. 2012
Received: 6 August 2012
Accepted: 5 November 2012
Published: 27 November 2012
The outstanding electrical and mechanical properties of graphene make it very attractive for several applications, Nanoelectronics above all. However a reproducible and non destructive way to produce high quality, large-scale area, single layer graphene sheets is still lacking. Chemical Vapour Deposition of graphene on Cu catalytic thin films represents a promising method to reach this goal, because of the low temperatures (T < 950°C−1000°C) involved during the process and of the theoretically expected monolayer self-limiting growth. On the contrary such self-limiting growth is not commonly observed in experiments, thus making the development of techniques allowing for a better control of graphene growth highly desirable. Here we report about the local ablation effect, arising in Raman analysis, due to the heat transfer induced by the laser incident beam onto the graphene sample.
KeywordsCVD graphene Copper Laser induced etching Heating ablation effects 61.80.Ba 81.15.Gh 61.48.Gh 81.05.ue
Graphene (a single bidimensional layer of carbon atoms arranged in an hexagonal lattice) has attracted a major interest in the last few years because of its astonishing electrical (Castro Neto et al.2009; Peres2010; Peres et al.2006), mechanical (Lee at al.2008) and chemical properties (Elias et al.2009; Wang et al.2009a), that make it a good candidate for the future development of nanoelectronics devices. Although the main properties of this material are nowadays well known from a theoretical point of view, an efficient and highly reproducible method to grow high quality, large-scale area, single layer graphene films, suitable for practical applications, is still lacking. For this reason, several techniques have been developed in the last years in order to achieve this goal: the most important are the epitaxial growth of graphene by thermal sublimation of SiC (de Heer et al.2007; Emtsev et al.2009; Hass et al.2008; Sprinkle et al.2009; Varchon et al.2007), the Chemical Vapour Deposition (CVD) synthesis of graphene on various metal catalysts (Reina et al.2009; Lee et al.2010; Liu et al.2010; Kim et al.2012; Nandamuri et al.2010; Somani et al.2006; Li et al.2009a;2009b; Tao et al.2012) and the chemical reduction of graphene oxide (Gilje et al.2007; Lee at al.2009; Paredes et al.2008; Schniepp et al.2006). Among these, CVD technique seems to be one of the most promising methods because of the reported possibility (Liu et al.2010) of obtaining highly uniform, defect-free graphene flakes as large as ∼ 100μ m2 in a reproducible, highly accessible and inexpensive way.
Since CVD synthesis needs a catalyst to activate the chemical decomposition of the carbon precursor (usually methane or ethylene) used for graphene growth at low temperatures (T < 950°C – 1000°C), the use of many metals (Ir (Coraux et al.2008), Ru (Martoccia et al.2008), Pt (Sasaki et al.2000; Starr et al.2006), Fe (Kondo et al.2010), Ag (Di et al.2008), Ni (Liu et al.2010; Kim et al.2009; Obraztsov et al.2007), Cu (Bae et al.2010; Li et al.2009a; Tao et al.2012) as catalysts during the process has been reported in literature. Cu is one of the most promising catalyst (Mattevi et al.2011) because of the low C solid solubility in it (0.001−0.008 weight % at ∼ 1084°C): this property brings to the formation of only soft (not covalent) bonds between the Π electrons of 2p z orbitals of sp2 hybridized C atoms and the 4s electrons of Cu, without formation of any carbide phase during the growth process. As a consequence, formation of graphene should stop after one single layer has been formed: this makes CVD growth of graphene on Cu very attractive. Nonetheless, many experiments show that actually such a self-limiting behaviour is hardly observed, since few-layered graphitic structures are usually grown on Cu substrates.
For this reason, to obtain monolayer graphene, several post processing techniques have been proposed to selectively etch atomic graphene layers. Among the various approaches (e.g. heat-induced etching by oxygen (Liu et al.2008), e-beam lithography assisted technique (Novoselov et al.2004; Zhang et al.2005), graphene cutting by carbon-soluble metals (Campos et al.2009; Datta et al.2008) the thinning of atomic carbon multilayers by laser irradiation (Han et al.2011) can be a promising method to obtain monolayer graphene. In this last work, authors show how the central rôle in graphene etching is held both by the laser irradiation used for the Confocal Raman Spectroscopy performed on the samples, and by the SiO2/Si substrate on top of which few-layered graphene has been transferred: the heat produced by the irradiation “burns” (in presence of oxygen) locally the outermost C layers, while the innermost layer (the one bound to the substrate) is left unetched because of the presence of the SiO2 layer acting as heat sink.
Cu, being a metal, has thermal conductivity higher than SiO2 and can represent therefore an enhanced heat sink, so it can be expected to observe a similar behaviour also for graphene grown by CVD on it.
Here we report the change in shape and position of the G and 2D peaks observed in Raman spectra acquired at different time intervals on the same spot of a graphene sample synthesized by CVD on Cu thin films: the evolution of the spectra, indicating that the structure of graphene is changing during the exposure to the laser used during Raman analysis, is compatible with a decrease in the number of graphene layers present on the substrate. This decrease may be attributed to the same laser-induced etching effect observed on graphene deposited onto SiO2/Si substrates. If this is the case, an efficient and easy graphene etching technique can be developed and a promising way to obtain high uniform, large-scale area, monolayer graphene can be envisaged.
The samples subjected to CVD process have been prepared by e-beam evaporation of 500 nm Cu thin film on top of a p-type (100) oriented Si wafer (∼ 1 cm2) with ∼ 300 nm thermal SiO2. The deposition has been carried out in a load-lock chamber at a base pressure of ∼ 10−8 mbar and deposition pressure of ∼ 10−6 mbar, with an average growth rate of 3−5 Å/s.
The thickness d of deposited Cu film has been chosen in order to limit the known problem (Mattevi et al.2011) of dewetting occurring on very thin films (d < 500 nm) at temperatures ≳ 800°C.
CVD growth process
The temperature of the system is controlled by a pyrometer, exposed to the back of the sample holder (a 4” Si wafer) and calibrated by means of a thermocouple in contact with it (Figure2). The pyrometer sets the power of the lamps. Since the Cu sample undergoing the CVD process is directly exposed to the lamps, the temperature reading by the pyrometer (correct in absence of Cu) is probably lower than the temperature reached by the surface during the process. Therefore, the real deposition temperature may be underestimated. We are performing some studies on this topic in order to solve this ambiguity in the future. However, at the temperature reached during the process as read by the pyrometer dissociation of CH4 and subsequent graphene formation take place, while the undesired Cu dewetting effect is prevented.
Graphene has been transferred from Cu to new insulating (285 nm-SiO2/Si) substrates by means of a standard chemical etching technique. Approximately 1.5 μ m of Poly(methyl-methacrylate) (PMMA) have been firstly deposited on graphene by spinning (at 5000 rpm for 1 minute) and heating (at 165°C for 5 minutes) the samples several times. After PMMA deposition, samples have been dipped in a 0.5 M diluted FeCl3 etching solution for ∼ 4 hours (keeping them at 45°C to enhance etching kinetics). Once Cu has been completely etched away from the samples, PMMA/graphene membranes have been picked up onto 285 nm-SiO2/Si substrates and PMMA has been finally removed with acetone.
Results and discussion
Graphene samples have been first characterized by SEM analysis and X-Ray Diffraction (XRD, performed with a Philips X’Pert Pro X-ray system using Co radiation beam at 0.8° incident angle) in order to investigate a change in granulometry and crystallographic orientation of the Cu surface, due to high temperature annealing under hydrogen flow.
Samples have been finally characterized with Raman spectroscopy by means of a Renishaw In-Via Raman Microscope, equipped with He-Cd blue laser at 442 nm, avoiding this way background plasmon emission of Cu when excited e.g. by green light (Tao et al.2012). For the acquisition we have used laser power both at 1 mW and 0.1 mW, by varying consequently the exposure time of the samples to laser irradiation (in order to keep the amount of energy E = Pt transferred from laser light to samples fixed).
It is possible to notice in particular that while the G peak shape and position are unaffected by laser exposure (only a slight increase in intensity is worthy of note), the D and 2D peaks change significantly their structure.
2D peak position and sharpness, I G /I 2D ratio
Graphene on Cu
Graphene on SiO 2
At such photon energies other mechanisms, like molecular desorption of chemical species, cannot be a priori excluded, but they can hardly affect the Raman signature and they can be detected through electrical measurements (Sun et al.2012).
The fact that the G peak position is almost unaffected by the laser irradiation can be explained as a result of two competing effects: the local enhancement of temperature (due to overheating), bringing to a redshift of the G peak (Cai et al.2010; Calizo et al.2007) and the decrease in the number of graphene layers (due to etching), resulting instead in a blueshift of the G peak (Wang et al.2009b).
The unexpected unaltered intensity of the G peak (that should decrease as the number of graphene layers decreases) can be explained in two ways. A first effect, applying to Raman measurements performed both on transferred and not transferred graphene samples, relies on the increase in temperature of graphene layers upon laser irradiation, likely resulting in an effect similar to what observed in experiments concerning the evolution of graphene Raman signature upon controlled annealing at high temperatures (Ni et al.2008a). As pointed out in this work, the G peak intensity is not changing between few- and monolayer graphene sheets after the annealing process, meaning that in these experimental conditions G peak intensity cannot be regarded as a fingerprint to distinguish number of graphene layers. A second reasoning, applying only on graphene samples over Cu, relies on the roughness of the Cu surface, determining a light trapping effect close to the substrate’s surface that results in an enhanced number of multiple reflections of the laser light between Cu and graphene layers: as a consequence, the number of C atoms detected by the unfocused beam is always comparable to the number of C atoms present in multilayer graphene, although the number of graphene layers is decreasing. As reported in (Ni et al.2008b) the G band intensity for a number of graphene layers exceeding ∼ 15 is in this case decreasing by increasing number of layers and then constant, as observed in our spectra.
The origin of the prominent D peak (increasing in intensity as the number of acquisitions increases) is not completely clear yet: it can be attributed to the acquisition of the spectra on a point of the sample lying on a grain boundary of the Cu substrate (resulting in a change of the crystallographic orientation of graphene flake through it) or to defects (terrace boundaries) produced in graphene crystal structure by the laser etching.
Raman analysis performed on transferred graphene samples using the same experimental setup (laser at 442 nm, power P = 1 mW and exposure time t = 80 s) confirms the behaviour observed in the spectra acquired on graphene/Cu substrates. A similar evolution in shape and position of the peaks is obtained for subsequent spectrum acquisitions, as shown in Figure7(b) and Figure8(b).
In summary, a possible way to locally etch graphene layers based on laser heating released during Raman analysis, has been presented. Graphene structure (crystallization degree and number of layers) evolution can be monitored and inferred by looking at the Raman spectra acquired on the sample. The technique is suitable in particular for etching layers of graphene grown by CVD on a metal catalyst. In our case we have reported results obtained with Cu: by lightening the sample with incident laser light at quite high power (≳ 1mW) for short time periods (∼ 80 s) a clear sharpening and lowering of the 2D peak position is observed in Raman spectra, together with a decrease in the IG/I2D ratio. These results are compatible with a decrease in the number of graphene layers grown on the metallic substrate. D peak increases in intensity as function of the laser exposure, meaning an increasing of defects in the graphene structure.
We believe that the method can be easily applied to other metallic substrates: since the technique deeply relies on the dispersion of the heat provided by laser irradiation through the substrate, the most important feature required for the substrate is its high thermal conductivity.
Although some catalysts, like Cu, are very promising for CVD synthesis of graphene because of the expected self-limited mono-layered growth of this material on them, a few-layered structure is often found in experiments. Laser etching here reported can therefore provide an in-situ technique to get rid of this problem. However, laser can also have an active rôle in inducing unwanted defects, such as vacancies in pristine graphene films: for this reason the proposed method shall be further developed. We finally envisage the application of the photo-etching process here reported to large areas if efficient and uniform illumination conditions, as those used in our RTA system, are employed.
Chemical vapour deposition
Scanning electron microscopy
Scanning tunneling microscopy
Root mean square
Atomic force microscopy
Rapid thermal annealing
The authors acknowledge the Nanofacility Piemonte and the Compagnia di San Paolo for financial supports. Thin films evaporation, graphene deposition and SEM analysis on the samples have been performed at Quantum Laboratories - Nanofacility Piemonte present at I.N.Ri.M. - Turin. Raman characterization has been performed with the help of A. Damin at the NIS Centre of Excellence - University of Turin. The help of A. Battiato and E. Olivetti with XPS and XRD analyses is gratefully acknowledge.
- Bae S, Kim H, Lee Y, Xu X, Park JS, Zheng Y, Balakrishnan J, Lei T, Kim HR, Song YI, Kim YJ, Kim KS, Özyilmaz B, Ahn JH, Hong BH, Iijima S: Roll-to-roll production of 30-inch graphene films for transparent electrodes. Nat Nanotechnol 2010, 5: 574-578.View ArticleGoogle Scholar
- Balandin AA, Ghosh S, Bao W, Calizo I, Teweldebrhan D, Miao F, Lau CN: Superior thermal conductivity of single-layer graphene. Nano Lett 2008, 8: 902-907. 10.1021/nl0731872View ArticleGoogle Scholar
- Cai W, Moore AL, Zhu Y, Li X, Chen S, Shi L, Ruoff RS: Thermal transport in suspended and supported monolayer graphene grown by chemical vapor deposition. Nano Lett 2010, 10: 1645-1651. 10.1021/nl9041966View ArticleGoogle Scholar
- Calizo I, Balandin AA, Bao W, Miao F, Lau CN: Temperature dependence of the raman spectra of graphene and graphene multilayers. Nano Lett 2007, 7: 2645-2649. 10.1021/nl071033gView ArticleGoogle Scholar
- Campos LC, Manfrinato VR, Sanchez-Yamagishi JD, Kong J, Jarillo-Herrero P: Anisotropic etching and nanoribbon formation in single-layer graphene. Nano Lett 2009, 9: 2600-2604. 10.1021/nl900811rView ArticleGoogle Scholar
- Castro Neto AH, Guinea F, Peres NMR, Novoselov KS, Geim AK: The electronic properties of graphene. Rev Mod Phys 2009, 81: 109-162. 10.1103/RevModPhys.81.109View ArticleGoogle Scholar
- Coraux J, N’Diaye AT, Busse C, Michely T: Structural coherency of graphene on Ir(111). Nano Lett 2008, 8: 565-570. 10.1021/nl0728874View ArticleGoogle Scholar
- Datta SS, Strachan DR, Khamis SM, Charlie Johnson A T: Crystallographic etching of few-layer graphene. Nano Lett 2008, 8: 1912-1915. 10.1021/nl080583rView ArticleGoogle Scholar
- de Heer WA, Berger C, Wu X, First PN, Conrad EH, Li X, Li T, Sprinkle M, Hass J, Sadowski ML, Potemski M, Martinez G: Epitaxial graphene. Solid State Commun 2007, 143: 92-100. 10.1016/j.ssc.2007.04.023View ArticleGoogle Scholar
- Di C, Wei D, Yu G, Liu Y, Guo Y, Zhu D: Patterned graphene as source/drain electrodes for bottom-contact organic field-effect transistors. Adv Mater 2008, 20: 3289-3293. 10.1002/adma.200800150View ArticleGoogle Scholar
- Elias DC, Nair RR, Mohiuddin TMG, Morozov SV, Blake P, Halsall MP, Ferrari AC, Boukhvalov DW, Katsnelson MI, Geim AK, Novoselov KS: Control of graphene’s properties by reversible hydrogenation: evidence for Graphane. Science 2009, 323: 610-613. 10.1126/science.1167130View ArticleGoogle Scholar
- Emtsev KV, Bostwick A, Horn K, Jobst J, Kellogg GL, Ley L, McChesney JL, Ohta T, Reshanov SA, Röhrl J, Rotenberg E, Schmid AK, Waldmann D, Weber HB, Seyller T: Towards wafer-size graphene layers by atmospheric pressure graphitization of silicon carbide. Nat Mater 2009, 8: 203-207. 10.1038/nmat2382View ArticleGoogle Scholar
- Ferrari AC, Meyer JC, Scardaci V, Casiraghi C, Lazzeri M, Mauri F, Piscanec S, Jiang D, Novoselov KS, Roth S, Geim AK: Raman spectrum of graphene and graphene layers. Phys Rev Lett 2006., 187401(1)–187401(4):Google Scholar
- Gilje S, Han S, Wang M, Wang KL, Kaner RB: A chemical route to graphene for device applications. Nano Lett 2007, 7: 3394-3398. 10.1021/nl0717715View ArticleGoogle Scholar
- Han GH, Chae SJ, Kim ES, Güneş F, Lee IH, Lee SW, Lee SY, Lim SC, Jeong HK, Jeong MS, Lee YH: Laser thinning for monolayer graphene formation: heat sink and interference effect. ACS Nano. 2011, 5: 263-268.Google Scholar
- de Heer WA, Conrad EH, Hass J: The growth and morphology of epitaxial multilayer graphene. J Phys-Condens Mat 2008, 20: 323202(1)-323202(27).Google Scholar
- Ismach A, Druzgalski C, Penwell S, Schwartzberg A, Zheng M, Javey A, Bokor J, Zhang Y: Direct chemical vapor deposition of graphene on dielectric surfaces. Nano Lett 2010, 10: 1542-1548. 10.1021/nl9037714View ArticleGoogle Scholar
- Kim H, Mattevi C, Calvo MR, Oberg JO, Artiglia L, Agnoli S, Hirjibehedin CF, Chhowalla M, Saiz E: Activation energy paths for graphene nucleation and growth on Cu. ACS Nano 2012, 6: 3614-3623. 10.1021/nn3008965View ArticleGoogle Scholar
- Kim KS, Zhao Y, Jang H, Lee SY, Kim JM, Kim KS, Ahn JH, Kim P, Choi JY, Hong BH: Large-scale pattern growth of graphene films for stretchable transparent electrodes. Nature 2009, 457: 706-710. 10.1038/nature07719View ArticleGoogle Scholar
- Kondo D, Sato S, Yagi K, Harada N, Sato M, Nihei M, Yokoyama N: Low-temperature synthesis of graphene and fabrication of top-gated field effect transistors without using transfer processes. Appl Phys Expr 2010, 3: 025102(1)-025102(3).Google Scholar
- Lee Y, Bae S, Jang H, Jang S, Zhu SE, Sim SH, Song YI, Hong BH, Ahn JH: Wafer-scale synthesis and transfer of graphene films. Nano Lett 2010, 10: 490-493. 10.1021/nl903272nView ArticleGoogle Scholar
- Lee CG, Park S, Ruoff RS, Dodabalapur A: Integration of reduced graphene oxide into organic field-effect transistors as conducting electrodes and as a metal modification layer. Appl Phys Lett 2009, 95: 023304(1)-023304(3).Google Scholar
- Lee C, Wei X, Kysar JW, Hone J: Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 2008, 321: 385-388. 10.1126/science.1157996View ArticleGoogle Scholar
- Li X, Cai W, An J, Kim S, Nah J, Yang D, Piner R, Velamakanni A, Jung I, Tutuc E, Banerjee SK, Colombo L, Ruoff RS: Large-area synthesis of high-quality and uniform graphene films on copper foils. Science 2009a, 324: 1312-1314. 10.1126/science.1171245View ArticleGoogle Scholar
- Li X, Cai W, Colombo L, Ruoff RS: Evolution of graphene growth on Ni and Cu by carbon isotope labeling. Nano Lett 2009b, 9: 4268-4272. 10.1021/nl902515kView ArticleGoogle Scholar
- Liu W, Chung CH, Miao CQ, Wang YJ, Li BY, Ruan LY, Patel K, Park YJ, Woo J, Xie YH: Chemical vapor deposition of large area few layer graphene on Si catalyzed with nickel films. Thin Solid Films 2010, 518: S128-S132. 10.1016/j.tsf.2009.10.070View ArticleGoogle Scholar
- Liu L, Ryu S, Tomasik MR, Stolyarova E, Jung N, Hybertsen MS, Steigerwald ML, Brus LE, Flynn GW: Graphene oxidation: thickness-dependent etching and strong chemical doping. Nano Lett 2008, 8: 1965-1970. 10.1021/nl0808684View ArticleGoogle Scholar
- Malard LM, Pimenta MA, Dresselhaus G, Dresselhaus MS: Raman spectroscopy in graphene. Phys Rep 2009, 473: 51-87. 10.1016/j.physrep.2009.02.003View ArticleGoogle Scholar
- Martoccia D, Willmott PR, Brugger T, Björck M, Günther S, Schlepütz CM, Cervellino A, Pauli SA, Patterson BD, Marchini S, Wintterlin J, Moritz W, Greber T: Graphene on Ru(0001): a 25×25 supercell. Phys Rev Lett 2008, 101: 126102(1)-126102(4).View ArticleGoogle Scholar
- Mattevi C, Kim H, Chhowalla M: A review of chemical vapor deposition of graphene on copper. J Mater Chem 2011, 21: 3324-3334. 10.1039/c0jm02126aView ArticleGoogle Scholar
- Miao C, Zheng C, Liang O, Xie YH: Chemical vapor deposition of graphene. In Physics and applications of graphene - experiments. Edited by: Mikhailov S. 2011. In Tech Rijeka, pp 37–54Google Scholar
- Nandamuri G, Roumimov S, Solanki R: Chemical vapor deposition of graphene films. Nanotechnology 2010, 21: 145604(1)-145604(4).View ArticleGoogle Scholar
- Ni ZH, Wang HM, Ma Y, Kasim J, Wu YH, Shen ZX: Tunable stress and controlled thickness modification in graphene by annealing. ACS Nano 2008a, 2: 1033-1039. 10.1021/nn800031mView ArticleGoogle Scholar
- Ni ZH, Wang YY, Yu T, Shen ZX: Raman spectroscopy and imaging of Graphene. Nano Res 2008b, 1: 273-291. 10.1007/s12274-008-8036-1View ArticleGoogle Scholar
- Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films. Science 2004, 306: 666-669. 10.1126/science.1102896View ArticleGoogle Scholar
- Obraztsov AN, Obraztsov EA, Tyurnina AV, Zolotukhin AA: Chemical vapor deposition of thin graphite films of nanometer thickness. Carbon 2007, 45: 2017-2021. 10.1016/j.carbon.2007.05.028View ArticleGoogle Scholar
- Paredes JI, Villar-Rodil S, Tascón JMD, Martínez-Alonso A: Graphene oxide dispersions in organic solvents. Langmuir 2008, 24: 10560-10564. 10.1021/la801744aView ArticleGoogle Scholar
- Peres NMR: The transport properties of graphene: an introduction. Rev Mod Phys 2010, 82: 2673-2700. 10.1103/RevModPhys.82.2673View ArticleGoogle Scholar
- Peres NMR, Guinea F, Castro Neto AH: Electronic properties of disordered two-dimensional carbon. Phys Rev B 2006, 73: 125411(1)-125411(23).Google Scholar
- Reina A, Jia X, Ho J, Nezich D, Son H, Bulovic V, Dresselhaus MS, Kong J: Large area, few-layer graphene films on arbitrary substrates by chemical vapor deposition. Nano Lett 2009, 9: 30-35. 10.1021/nl801827vView ArticleGoogle Scholar
- Sasaki M, Yamada Y, Ogiwara Y, Yagyu S, Yamamoto S: Moiré contrast in the local tunneling barrier height images of monolayer graphite on Pt(111). Phys Rev B 2000, 61: 15653-15656. 10.1103/PhysRevB.61.15653View ArticleGoogle Scholar
- Schniepp HC, Li JL, McAllister MJ, Sai H, Herrera-Alonso M, Adamson DH, Prud’homme RK, Car R, Saville DA, IAv Aksay: Functionalized single graphene sheets derived from splitting graphite oxide. J Phys Chem B 2006, 110: 8535-8539.View ArticleGoogle Scholar
- Somani PR, Somani SP, Umeno M: Planes nano-graphenes from camphor by CVD. Chem Phys Lett 2006, 430: 56-59. 10.1016/j.cplett.2006.06.081View ArticleGoogle Scholar
- Sprinkle M, Siegel D, Hu Y, Hicks J, Tejeda A, Taleb-Ibrahimi A, Le Févre P, Bertran F, Vizzini S, Enriquez H, Chiang S, Soukiassian P, Berger C, de Heer WA, Lanzara A, Conrad EH: First direct observation of a nearly ideal graphene band structure. Phys Rev Lett 2009, 103: 226803(1)-226803(4).View ArticleGoogle Scholar
- Starr DE, Pazhetnov EM, Stadnichenko AI, Boronin AI, Shaikhutdinov SK: Carbon films grown on Pt(111) as supports for model gold catalysts. Surf Sci 2006, 600: 2688-2695. 10.1016/j.susc.2006.04.035View ArticleGoogle Scholar
- Su CY, Lu AY, Wu CY, Li YT, Liu KK, Zhang W, Lin SY, Juang ZY, Zhong YL, Chen FR, Li LJ: Direct formation of wafer scale graphene thin layers on insulating substrates by chemical vapor deposition. Nano Lett 2011, 11: 3612-3616. 10.1021/nl201362nView ArticleGoogle Scholar
- Sun PZ, Zhu M, Wang KL, Zhong ML, Wei JQ, Wu DH, Cheng Y, Zhu HW: Photoinduced molecular desorption from graphene films. Appl Phys Lett 2012, 101: 053107(1)-053107(4).Google Scholar
- Tao L, Lee J, Chou H, Holt M, Ruoff RS, Akinwande D: Synthesis of high quality monolayer graphene at reduced temperature on hydrogen-enriched evaporated copper (111) films. ACS Nano 2012, 6: 2319-2325. 10.1021/nn205068nView ArticleGoogle Scholar
- Varchon F, Feng R, Hass J, Li X, Ngoc Nguyen B, Naud C, Mallet P, Veuillen JY, Berger C, Conrad EH, Magaud L: Electronic structure of epitaxial graphene layers on SiC: effect of the substrate. Phys Rev Lett 2007, 99: 126805(1)-126805(4).View ArticleGoogle Scholar
- Wang X, Li X, Zhang L, Yoon Y, Weber PK, Wang H, Guo J, Dai H: N-Doping of graphene through electrothermal reactions with ammonia. Science 2009a, 324: 768-771. 10.1126/science.1170335View ArticleGoogle Scholar
- Wang H, Wang Y, Cao X, Feng M, Lan G: Vibrational properties of graphene and graphene layers. J Raman Spectrosc 2009b, 40: 1791-1796. 10.1002/jrs.2321View ArticleGoogle Scholar
- Zhang Y, Tan YW, Stormer HL, Kim P: Experimental observation of the quantum hall effect and Berry’s phase in graphene. Nature 2005, 438: 201-204. 10.1038/nature04235View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.